semicrystalline thermoplastic elastomeric polyolefins ... thermoplastic elastomeric polyolefins:...
Embed Size (px)
Semicrystalline thermoplastic elastomeric polyolefins:Advances through catalyst development andmacromolecular designAtsushi Hotta*†, Eric Cochran*‡, Janne Ruokolainen*§, Vikram Khanna*, Glenn H. Fredrickson*¶, Edward J. Kramer*¶,Yong-Woo Shin�, Fumihiko Shimizu�, Anna E. Cherian**, Phillip D. Hustad**††, Jeffrey M. Rose**,and Geoffrey W. Coates¶**
*Mitsubishi Chemical Center for Advanced Materials and Departments of Materials and Chemical Engineering, University of California,Santa Barbara, CA 93106; �Mitsubishi Chemical Group, Science and Technology Research Center, Inc., 1000 Kamoshida-cho, Aoba-ku,Yokohama 227-8502, Japan; and **Department of Chemistry and Chemical Biology, Baker Laboratory, Cornell University, Ithaca, NY 14853
Edited by Tobin J. Marks, Northwestern University, Evanston, IL, and approved July 10, 2006 (received for review April 20, 2006)
We report the design, synthesis, morphology, phase behavior,and mechanical properties of semicrystalline, polyolefin-basedblock copolymers. By using living, stereoselective insertionpolymerization catalysts, syndiotactic polypropylene-block-poly(ethylene-co-propylene)-block-syndiotactic polypropyleneand isotactic polypropylene-block-regioirregular polypropylene-block-isotactic polypropylene triblock copolymers were synthe-sized. The volume fraction and composition of the blocks, as wellas the overall size of the macromolecules, were controlled bysequential synthesis of each block of the polymers. These triblockcopolymers, with semicrystalline end-blocks and mid-segmentswith low glass-transition temperatures, show significant potentialas thermoplastic elastomers. They have low Young’s moduli, largestrains at break, and better than 90% elastic recovery at strainsof 100% or less. An isotactic polypropylene-block-regioirregularpolypropylene-block-isotactic polypropylene-block-regioirregularpolypropylene-block-isotactic polypropylene pentablock copoly-mer was synthesized that also shows exceptional elastomericproperties. Notably, microphase separation is not necessary inthe semicrystalline isotactic polypropylenes to achieve good me-chanical performance, unlike commercial styrenic thermoplasticelastomers.
block copolymer � polypropylene
The applications of a polymer are largely determined by itschemical, physical, and mechanical properties. These prop-
erties are in turn determined by polymer morphology, which isdictated by polymer structure and composition. Thermoplasticelastomers are a classic example where polymer architectureengenders unique properties. Block copolymers that contain atleast two blocks that are hard at room temperature, separated byblocks with a glass transition temperature (Tg) below roomtemperature, typically exhibit elastomeric properties if the low Tgblock volume is large (1–5). The most well known elastomers ofthis type are the polystyrene (PS)-block (b)-polybutadiene-b-PStriblock copolymers, sold commercially by Kraton Polymers.Such materials normally possess a microphase-separated mor-phology in which 10-nm-scale domains of the hard blocks (e.g.,PS) are embedded as spheres or cylinders within a continuousphase of the low Tg soft blocks. The hard domains serve asthermally reversible crosslinks that at room temperature pro-duce high levels of recoverable elasticity in the soft phase.
Sequence control of a synthetic polymer is most easily accom-plished by using a synthetic technique that allows the sequentialaddition of one or more monomers to the macromolecule in achain growth process without spontaneous termination. Thesetechniques are collectively called living polymerizations, anddespite many successes over the last half century, their furtherdevelopment remains one of the most important frontiers inpolymer science. In the case of the Kraton triblock copolymers,
a living anionic polymerization process is used to synthesize thematerials. Because approximately two-thirds of all thermoplasticpolymers are polyolefins, a significant amount of research hasbeen directed toward the development of living catalysts foralkene polymerization. Living catalysts enabling the synthesis ofblock olefin copolymers have only been popularized in the lastdecade (6).
Block PolyolefinsThere are two main ways to produce polyolefins with blockystructures: (i) use nonliving alkene polymerization catalysts,where changes at the site of enchainment during chain formationgives rise to different blocks in the polymer; and (ii) employliving catalysts, and change the monomer or reaction conditionsduring chain formation resulting in controlled block formation.The first approach has the advantage that more than one chainis formed per catalyst center but has the disadvantage thatprecise control of the number and length of blocks is not easilyaccomplished. Some examples of nonliving catalysts that pro-duce olefin-based block copolymers include heterogeneousZiegler-Natta catalysts (7), asymmetric metallocenes (8, 9), andthe oscillating metallocenes (10). Although living catalysts havethe inherent disadvantage that they typically only produce onechain per catalytic active center, they do have the potential forunprecedented levels of control of polymer architecture, includ-ing the composition, size, and number of blocks in olefincopolymers (6). Regarding thermoplastic elastomers, they allowthe precise placement of hard blocks of high melting point (Tm)or Tg, and soft blocks of Tg well below ambient temperature.Because of the widespread use of ethylene and propylene asmonomers for the synthesis of polyolefins, these monomers areprime candidates for feedstocks for thermoplastic elastomersynthesis. Isotactic or syndiotactic polypropylene (iPP or sPP)blocks, as well as linear polyethylene (PE) blocks, are obvious
Conflict of interest statement: No conflicts declared.
This article is a PNAS direct submission.
Abbreviations: b, block; iPP, isotactic PP; PEP, poly(ethylene-co-propylene); PP, polypro-pylene; PS, polystyrene; rPP, regioirregular PP; SEBS, PS-b-poly(ethylene-co-butylene)-b-PS;sPP, syndiotactic polypropylene; TEM, transmission electron microscopy.
†Present address: Department of Mechanical Engineering, Keio University, 3-14-1 HiyoshiKohoku-ku, Yokohama 223-8522, Japan.
‡Present address: Department of Chemical and Biological Engineering, Iowa State Univer-sity, Ames, IA 50011.
§Present address: Department of Engineering Physics, Helsinki University of Technology,P.O. Box 2200, FIN-02015, Helsinki, Finland.
††Present address: Polyolefins and Elastomers R&D, Dow Chemical Company, 2301 NorthBrazosport Boulevard, B-3814, Freeport, TX 77541.
© 2006 by The National Academy of Sciences of the USA
www.pnas.org�cgi�doi�10.1073�pnas.0602894103 PNAS � October 17, 2006 � vol. 103 � no. 42 � 15327–15332
choices for the hard blocks, although tactic PP segments arepotentially advantaged because of their higher melting temper-atures and greater resistance to chain pullout from crystals. Forthe soft segments, random, amorphous poly(ethylene-co-propylene) (PEP) copolymer blocks are superior to atactic PPsegments because of their significantly lower Tg values (approx-imately �50 versus 0°C).
Few catalysts exhibit living behavior for both the synthesis oftactic PPs and amorphous PEPs. Living, partially syndiotactic PPwas first reported by Doi (11) using vanadium complexes. Coates(12) and Fujita (13) independently reported that fluorinatedbis(phenoxyimine) titanium catalysts (14) are capable of theliving, syndiospecific polymerization of propylene, including thesynthesis of polymers with PEP blocks. Busico (15), Coates (16),and Sita (17) have reported group IV catalysts with varyingdegrees of isospecificity and livingness for the synthesis of iPPblock copolymers. Notably, Sita (17) has recently reported thesynthesis of elastomeric multiblock polymers with atactic PP andiPP segments. Coates (18) has recently reported a chiral nickelalpha-diimine catalyst that produces di- and elastomeric triblockpolypropylenes with isotactic and regioirregular (rPP) PP blocks,controlled by the polymerization temperature. A possible ad-vantage of this system is that rPP blocks are virtually indistin-guishable from PEP blocks and have a suitably low Tg ofapproximately �55°C, enabling the synthesis of thermoplasticelastomers from a single monomer.
The focus of this article is the synthesis of thermoplastic elas-tomers from ethylene and propylene by using stereoselective, livingalkene polymerization catalysts. Specifically, a titanium catalyst (1;
Fig. 1) was used to synthesize a sPP-b-PEP-b-sPP triblock copoly-mer (synTB) by a sequential polymerization procedure (Scheme 1).A chiral nickel catalyst (2; Fig. 1) was used to synthesize aniPP-b-rPP-b-iPP triblock copolymer (isoTB) and an iPP-b-rPP-b-iPP-b-rPP-b-iPP pentablock copolymer (isoPB; Scheme 1). Herein,we show that the design and precision control of polymer structureallows for the synthesis of thermoplastic elastomeric polyolefinswith unprecedented properties.
Results and DiscussionPolymer Design. Our objective in this project was to develop olefinblock copolymers that could be used as thermoplastic elastomersand potentially be competitive, in cost and performance, withhydrogenated styrenic block copolymers and thermoplastic ure-thane elastomers. Given the limited data on olefin block copol-ymer systems, we attempted a design based on our experiencewith styrenic block copolymer elastomers. In particular, wefocused primarily on triblock copolymers with two semicrystal-line end blocks (‘‘hard’’ blocks) and an internal amorphous,low-Tg, ‘‘soft’’ block. (In the case of PEP soft blocks, an ethylenemole fraction between 0.4 and 0.7 is desirable to produce a lowTg and avoid crystallization.) We also prepared and tested apentablock copolymer with a linear hard–soft–hard–soft–hardstructure. It was our expectation that good elastic recoverywould require block copolymer mesophases with a continuoussoft domain and discrete hard domains. Thus, we aimed forsamples with 20–30% by volume of the hard blocks. In the caseof styrenic elastomers, which have glassy PS hard blocks, goodperformance mandates that the molecular weight be adjusted sothat the order–disorder transition (TODT) (2) satisfies the in-equality Tuse � Tg � TODT. This ensures that upon cooling froma melt processing temperature Tproc, block mesophases areformed before vitrification at Tg, resulting in a well orderedelastomer with glassy (and nearly pure) PS domains at theapplication temperature Tuse. Ideally, for ease of processing onewould like TODT � Tproc, although this is often not possible inhydrogenated PS block copolymers because of the large Flory �parameter between PS segments and PEP or poly(ethylene-co-butylene) segments.
Adapting these design rules to the sPP block copolymers, weinitially targeted ‘‘symmetric’’ sPP-b-PEP-b-sPP triblock copol-ymers with equal-length sPP blocks and overall molecular weight(�350 K) consistent with the sequence Tuse � Tm � TODT �
Fig. 1. Catalyst precursors for the synthesis of tactic PP block copolymers.
Scheme 1. Synthesis of synTB, isoTB, and isoPB.
15328 � www.pnas.org�cgi�doi�10.1073�pnas.0602894103 Hotta et al.
Tproc. Such materials form ordered mesophases in the melt uponcooling, and the subsequent crystallization is then confined tothe sPP-rich minority domains. For reasons of synthetic conve-nience, the iPP-b-rPP-b-iPP triblock and iPP-b-rPP-b-iPP-b-rPP-b-iPP pentablock copolymers were prepared at significantlylower overall molecular weight (�150 K), which implies theinverted sequence (Tuse, TODT) � Tm � Tproc. In these cases,crystallization occurs upon cooling from the disordered melt, soany subsequent TODT is unobservable. Because the iPP blockcopolymers did not possess the ideal thermal sequence based onstyrenic block copolymer design, we expected that they would beinferior mechanically to the sPP block copolymers. As will bediscussed below, this naı̈ve expectation turned out to be incorrectand has highlighted an important design advantage of semicrys-talline block copolymers over their amorphous counterparts.
Polymer Synthesis. Two different classes of polyolefin-based blockcopolymer systems were prepared. The first consists of blocks ofsyndiotactic polypropylene (sPP) and ethylene-propylene ran-dom copolymer (PEP). Fig. 1 shows the catalyst structure andScheme 1 the synthetic scheme for synthesizing the block co-polymers. Polymerization of propylene at 0°C resulted in a livingpolymerization of sPP ([rrrr] � 0.96). Once a block of the desiredlength was grown, a slight overpressure of ethylene was addedand polymerized to produce a PEP block (12, 19). Triblockcopolymers of sPP-b-PEP-b-sPP were synthesized by a similarprocedure by adding a final polymerization of pure PP to thesequence. The sPP had a melting temperature between 130 and146°C, decreasing with increasing molecular weight (19). Forethylene fractions (Fe) greater than 0.75 in the PEP block,crystallization of PE segments in the PEP could be detected.Synthesis of sPP-b-PE in which both blocks are semicrystallinewas possible (19), although these were not good thermoplasticelastomers and were not considered further. The second poly-olefin-based block copolymer system consists of blocks of iPPand rPP. Fig. 1 shows the catalyst structure and Scheme 1 thesynthetic scheme for this block copolymer. In this case, pro-pylene is the only monomer. When the polymerization temper-ature is �60°C or lower, iPP results, whereas at room temper-ature, the incorporation of trimethylene units [O(CH2)3O]predominates. These unbranched units are due to 3,1-insertionsarising from catalyst chain-walking (18). The rPP block thatresults at 0°C resembles PEP (nominal Fe � 0.53) more than itdoes PP and in fact has a glass transition temperature (less than�40°C) that is much lower than conventional amorphous PP. Asthe polymerization temperature is decreased, the effective Fedecreases (0.11 at �60°C and 0 at �78°C), although the poly-merization rate decreases dramatically. Triblock and pentablockcopolymers can be produced simply by carrying out sequentialpolymerizations at different temperatures.
Polymer Morphology and Mechanical Testing. The morphology ofthe polyolefin block copolymers produced by these methods was
determined by transmission electron microscopy (TEM) usingRuO4 to stain the amorphous regions and in selected cases byscanning force microscopy. Order–disorder transition temper-atures in the melt (TODT) were determined by dynamic mechan-ical spectroscopy (19). Mechanical testing was performed intension by sequentially loading and unloading, measuring thehysteresis loop and the strain not recovered after unloading.Triblock sPP-b-PEP-b-sPP copolymers. Triblock copolymers of sPP-b-PEP-b-sPP with relatively low sPP contents (weight fractions wPP� 0.3) and Fe in the PEP block �0.7 have excellent propertiesas thermoplastic elastomers. An example is a triblock copolymerwith 25 wt % sPP, a total number average molecular weight (Mn,tot) of 298 kg�mol, and Fe � 0.66 (synTB; Table 1). synTB has amicrophase-separated morphology consisting of sPP cylinders ina PEP matrix as shown in the TEM micrograph in Fig. 2. Theroom temperature stress–strain curve for this block copolymershown in Fig. 3 is elastomeric with an initial Young’s modulus of�7 MPa and a strain-to-break of �550%. Similar results werefound at an elevated testing temperature of 65°C. The elasticrecovery (the fraction of the maximum applied strain recoveredright after unloading) is plotted as a function of maximum strainin Fig. 4.
At maximum strains of 100% or less, the elastic recovery isbetter than 90%. These properties are comparable with or betterthan those of commercial PS-b-poly(ethylene-co-butylene)-b-PS(SEBS) triblock copolymers with cylindrical PS microstructures.The elastic recovery is nearly 100% in the second and subsequentcycles as long as the original maximum strain is not exceeded. As
Table 1. Characterization of semicrystalline block copolymers
Wt. % ofhard blocks†
Fe in softblocks‡ Tm, °C§ Tg, °C§
sPP-b-PEP-b-sPP (synTB) 298 1.20* 37–225–36* 24 0.66 36, 134 �57iPP-b-rPP-b-iPP (isoTB) 109 1.14¶ 10–83–16¶ 24 0.53 130 �44iPP-b-rPP-b-iPP-b-rPP-b-iPP (isoPB) 159 1.39¶ 16–75–6–46–16¶ 24 0.53 125 �46
*Determined by using gel-permeation chromatography in 1,2-C6H4Cl2 at 135°C versus polypropylene standards.†Wt. % of hard blocks � (� Mn, hard)�(Mn, tot).‡Mole fraction of ethylene in PEP block (Fe) determined by 13C NMR. Mole fraction of ethylene (Fe) in rPP block(s) determined by usingthe PP formed at 0°C by the equation: Fe � [(1 � R)�(1 � R)], and R � [CH3]�[CH2], determined by 1H NMR.
§Determined by differential scanning calorimetry (second heat).¶Determined by using gel-permeation chromatography in 1,2,4-C6H3Cl3 at 140°C versus polyethylene standards.
Fig. 2. TEM micrograph of synTB (sPP cylinders are white).
Hotta et al. PNAS � October 17, 2006 � vol. 103 � no. 42 � 15329
expected, triblock copolymers with larger sPP contents (wPP �0.5) and comparable Mn, tot have microphase-separated micro-structures with continuous sPP domains. While these showstrains at break that exceed 500%, they also have significantlylarger Young’s moduli, yield behavior, and poor elastic recoverydue to extensive plastic deformation of the sPP phase.Triblock iPP-b-rPP-b-iPP copolymers. Triblock iPP-b-rPP-b-iPP copol-ymers show even more interesting mechanical properties. As canbe seen in Fig. 5, TEM analysis of an iPP-b-rPP-b-iPP blockcopolymer, sample isoTB (Table 1), shows no evidence ofmicrophase separation, a finding that is consistent with itsrelatively low total molecular weight (109 kg�mol) and the loweffective ethylene content of its rPP mid-block (19). Crystals ofiPP (white) can be seen throughout the TEM image. Despite itslack of microphase separation, the elastomeric properties of thesample are exceptional. Its Young’s modulus is less than half thatof the sPP-b-PEP-b-sPP block copolymer, synTB, and its strain-to-break, over 1,700%, is over three times higher (Fig. 3). In
addition, it shows very good elastic recovery out to 1,000% strainas shown in Fig. 4. At a testing temperature of 65°C, the Young’smodulus of sample isoTB is nearly identical to the room tem-perature value, as is its elastic recovery up to a strain at breakof 400%.
In comparison, a microphase-separated SEBS of comparabletotal molecular weight (96 kg�mol) and wt % hard block (28%PS) has (at room temperature) a Young’s modulus of 9 MPa, astrain to failure of 500%, and an elastic recovery of only 78%after a maximum strain of 100%. At a testing temperature of65°C, the SEBS has a strain at break of 200% and an elasticrecovery of �80%. The iPP-b-rPP-b-iPP sample, isoTB, not onlyhas superior elastomeric properties but is much easier to processthan SEBS because of the lack of microphase separation in themelt state.Pentablock iPP-b-rPP-b-iPP-b-rPP-b-iPP copolymers. As a final example,an iPP-b-rPP-b-iPP-b-rPP-b-iPP pentablock copolymer was pre-pared with 21 wt % iPP and Mn, tot � 159 kg�mol (isoPB; Table1). As with its triblock counterpart isoTB, TEM analysis of isoPBshows no evidence of microphase separation, only white crystalsof iPP (Fig. 6). The mechanical properties at room temperatureare truly exceptional with a strain at break of 2,400% and amaximum tensile true stress of 250 MPa before break (Fig. 3).Although the elastic recovery of isoPB is lower than that of isoTBat strains of 10% and 50%, perhaps because of increasing crystalconnectivity resulting from shorter rPP blocks, it rises to a valueof nearly 90% out to strains of 1,000%, almost identical to isoTB(Fig. 4). The pentablock architecture (20), with an internal hardblock, is apparently very effective at thwarting chain pulloutfrom crystals at high levels of stress.
The temperature range over which these sPP and iPP blockcopolymers will exhibit good elastomeric properties should belimited at the low end by the glass transition temperature ofthe mid-block (less than �40°C) and on the upper end by thetemperature at which the end blocks can be pulled free of thecrystals anchoring them. The iPP blocks appear to be superiorhard blocks, possibly because it is harder to remove an iPP chainfrom a crystal, and the middle iPP block of the pentablock alsoappears to thwart chain pullout. The low Tg of the soft blocksshould lead to a significant improvement of low-temperatureproperties over atactic–isotactic stereoblock polypropylenes (10,
Fig. 3. Tensile true stress-versus-strain curves for synTB, isoTB, and isoPB.
Fig. 4. Elastic recovery of synTB, isoTB, and isoPB as a function of maximumtensile strain.
Fig. 5. TEM micrograph of isoTB showing iPP crystals but no microphaseseparation.
15330 � www.pnas.org�cgi�doi�10.1073�pnas.0602894103 Hotta et al.
17), which have a Tg of �0°C. Because the melting temperatureof the iPP block in isoTB is only 130°C, probably limited byoccasional 3,1-insertions that introduce O(CH2)3O units intothe iPP block, development of new catalysts that will improve theregioregularity of that block should lead to improvement inhigh-temperature strain-to-break and elastic recovery.
ConclusionsThe advent of advanced catalysts for polyolefin synthesis thatoffer simultaneous control over molecular weight, stereochem-istry, and chain termination processes has created a significantopportunity for the design of entirely new classes of polyolefinmaterials based on block copolymer architectures. Given the lowcost and wide availability of olefinic monomers, coupled with thebroad range of materials properties achievable with these newcatalysts, it would seem that the area is ripe for further research,development, and commercialization.
The present work has explored only one small sector ofmaterials design space: semicrystalline polyolefin block copoly-mers for use as thermoplastic elastomers. Nonetheless, we haveshown the potential of polyolefin block copolymers in this sectorby achieving elastomeric properties in sPP and iPP systems thatrival or exceed those of commercial SEBS thermoplastic elas-tomers. Moreover, the polyolefin elastomers offer a consider-able advantage in melt processibility, monomer cost, and po-tentially high-temperature performance and chemical andsolvent resistance.
An important outcome of our work is that the design rules forelastomers based on semicrystalline hard blocks are more for-giving than those for traditional amorphous thermoplastic elas-tomers such as SEBS. The large enthalpy of crystallizationoverwhelms the small favorable free energy of segment mixingin low-molecular-weight block copolymers at Tm, producing arandom crystal morphology with no short- or long-range orderon the mesoscale. Surprisingly, this disordered morphology canpossess excellent elastomeric properties that exceed those ofeven well microphase-separated materials. Thus, in contrast toelastomers that use glassy hard blocks, it is not necessary tomaintain a high molecular weight to ensure TODT � Tm. Thisdesign flexibility should allow the rheological and mechanical
properties of semicrystalline thermoplastic elastomers to betuned over a much broader range.
Major challenges remaining are catalyst cost, recovery, andproductivity, which are particularly acute impediments to com-mercialization of polymers based on living polyolefin catalysts.Now that the potential property advantages of block polyolefinmaterials are clear, we are optimistic that there will be a strongincentive to overcome these difficulties in both living andnonliving catalyst systems.
Materials and MethodsPolymer Synthesis. Complexes 1 and 2 were synthesized as pre-viously reported (12, 18).Synthesis of sPP-b-PEP-b-sPP (synTB). A 2-liter stainless steel auto-clave was charged with PMAO (1.20 g, 20.8 mmol Al) andtoluene (1 liter) under nitrogen atmosphere. The reactor wascooled to 0°C, and the atmosphere was exchanged with pro-pylene gas and then saturated under pressure [2.0 atm (1 atm �101.3 kPa)]. A solution of titanium complex 1 (90 mg, 0.10 mmol)in toluene (7 ml) was then added to the reactor via gas-tightsyringe to initiate the polymerization. After 35 h, the unreactedpropylene monomer was removed with a vacuum pump, themixture of ethylene and propylene (32�68 mol/mol, 0.68 atm)was introduced into the reactor, and the mixture of the gas wasfed to keep the pressure constant at 0.68 atm. After an additional0.42 h, the feed of the mixed gas was stopped and the unreactedmonomer gas was removed with a vacuum pump. The polymer-ization was allowed to continue in the presence of propylene (1.4atm) for an additional 35 h. The reaction was then quenched byinjection of methanol�HCl (25 ml, 10% vol HCl). After ventingthe reactor, the polymer was precipitated in copious methanol�HCl, filtered, washed with methanol, and dried in vacuo toconstant weight (25 g).Synthesis of iPP-b-rPP-b-iPP (isoTB). A 6-oz Lab-Crest pressure reac-tion vessel equipped with a magnetic stir bar was charged withMMAO-3A (2.5 ml of a 7-wt % solution in heptane, 4 mmol Al)and toluene (30 ml) in a nitrogen-filled glovebox. The reactorwas cooled to �60°C, the atmosphere was exchanged withpropylene gas three times, and the flask was filled with 30 g ofpropylene. A solution of nickel complex 2 (17.4 mg, 0.017 mmol)in CH2Cl2 (2 ml) was then added to the reactor via gas-tightsyringe to initiate the polymerization. After 38 h, a 2-ml samplewas removed via cannula and the flask was warmed to 0°C. Afterstirring an additional 3.5 h, another 2-ml sample was removed,and the polymerization was cooled to �60°C and allowed tocontinue for an additional 76 h. The reaction was then quenchedby injection of methanol�HCl (5 ml, 10% vol HCl). After ventingthe reactor, the polymer was precipitated in copious methanol�HCl, filtered, washed with methanol, and dried in vacuo toconstant weight (2.45 g).Synthesis of iPP-b-rPP-b-iPP-b-rPP-b-iPP (isoPB). A 6-oz Lab-Crestpressure reaction vessel was prepared as described above forisoTB to generate the first iPP block. After 48 h at �60°C, a 2-mlsample was removed via cannula and the flask was warmed to0°C. After stirring an additional 2 h, another 2-ml sample wasremoved and the polymerization was cooled to �60°C andallowed to continue. After 48 h, a 2-ml sample was removed viacannula and the flask was warmed to 0°C. After stirring anadditional 2 h, another 2-ml sample was removed, and thepolymerization was cooled to �60°C and allowed to continue foran additional 66 h. The reaction was then quenched by injectionof methanol�HCl (5 ml, 10% vol HCl). After venting the reactor,the polymer was precipitated in copious methanol�HCl, filtered,washed with methanol, and dried in vacuo to constant weight(2.16 g).
At each stage of the polymerization, molecular weights weredetermined by removing an aliquot of the polymer and subjectingit to gel-permeation chromatography at elevated temperature.
Fig. 6. TEM micrograph of isoPB showing iPP crystals but no microphaseseparation.
Hotta et al. PNAS � October 17, 2006 � vol. 103 � no. 42 � 15331
Transmission Electron Microscopy. All samples for TEM wereannealed in the melt for a total of 7 days, the first 4 days at 200°Cto erase any previous thermal history and then an additional 3days at a final temperature of 160°C. High-vacuum ovens [�10�7
mbar (1 bar � 100 kPa)] were used to prevent degradation byoxidation. Melt morphology was preserved by quickly quenchingthe samples after annealing. TEM images of quenched sampleswere recorded at 200 kV with either a JEOL (Tokyo, Japan)2000FX or an FEI (Hillsboro, OR) Technai T-20 TEM. Thecontrast for the morphological characterization was achieved bya sample preparation technique that relies on different rates ofdiffusion of a RuO4 stain into the amorphous and semicrystallineregions (21). First, the sample surface was cut at �170°C to makea smooth surface for the stain to penetrate into the sample. Thesamples were then stained in a vapor of a 0.5% RuO4 stabilizedaqueous solution (Electron Microscopy Sciences, Fort Washing-ton, PA) for a period of between 5 and 7 days. The stainedsample was microtomed by using a Leica (Deerfield, IL) UltracutUCT ultramicrotome with a diamond knife at room tempera-ture, and 80-nm-thick sections were collected on 600-meshhexagonal grids.
Differential Scanning Calorimetry. Polymer melting point (Tm) andglass transition temperature (Tg) were measured by differentialscanning calorimetry with a TA Instruments (New Castle, DE)Q1000 calorimeter equipped with an automated sampler. Anal-yses were performed in crimped aluminum pans under nitrogen,and data were collected from the second heating run at a heatingrate of 10°C�min from �100 to 200°C and processed with TAInstruments Q Series software.
Tensile Mechanical Testing. After the synthesis, powder materialswere compression-molded into a small film �0.2 mm thick. Filmsamples were then moved into a high-vacuum oven to beannealed for 4 days (the first day at 200°C and the remaining 3
days at 160°C). After annealing, samples were cut into rectan-gular specimens �7.5 mm long, 1 mm wide, and 0.2 mm thick.Cut samples were then either stretched to fracture or up to agiven tensile strain � using an Instron (Norwood, MA) 1123testing machine. All testing was performed at room temperature(�20°C). The strain rate was held constant at �0.01�s. Two typesof mechanical tests were performed as follows. (i) Samples werestretched monotonically to fracture, and stress–strain curveswere recorded. True stresses were computed by correctingmeasured nominal stress values for the specimen area decreaseat large tensile strains. (ii) Step cycle tests were performed thatcombine a stepwise stretching of the rectangular samples withunloading–reloading cycles. In each step, the sample was ex-tended step by step up to strains of 10, 50, 100, 250, 500, and 750(%). Once the sample reached the appropriate strain, thecrosshead direction was reversed and the sample strain wasdecreased at the same rate until zero stress was achieved. Thesample was then extended again at the same constant strain rateuntil it reached the next targeted step-strain. The step cycle testwas performed until the sample fractured or until the final stepof 750% was reached. With this step cycle test, we measured theelastic recovery of the materials. The elastic recovery R(%) isdefined as the strain recovered upon unloading divided by themaximum strain reached during the step.
We thank the Mitsubishi Chemical Corporation for financial support ofthis research. This work made use of MRL Central Facilities at the Uni-versity of California, Santa Barbara, which are supported by the Mate-rials Research Science and Engineering Centers Program of the NationalScience Foundation under Award DMR-0520415, and of the CornellCenter for Materials Research Shared Experimental Facilities, which aresupported by the Materials Research Science and Engineering CentersProgram of the National Science Foundation under Award DMR-0520404. This material is based on work supported in part by the U.S.Army Research Laboratory and the U.S. Army Research Office underGrant DAAD19-02-1-0275 (Macromolecular Architecture for Perfor-mance, Multidisciplinary University Research Initiative).
1. Holden G, Kricheldorf HR, Quirk RP (2004) Thermoplastic Elastomers(Hanser, Munich).
2. Bates FS (1991) Science 251:898–905.3. Hamley IW (1998) The Physics of Block Copolymers (Oxford Univ Press,
Oxford).4. Lodge TP (2003) Macromol Chem Phys 204:265–273.5. Ruzette AV, Leibler L (2005) Nat Mater 4:19–31.6. Coates GW, Hustad PD, Reinartz S (2002) Angew Chem Int Ed 41:2236–2257.7. Collette JW, Tullock CW, MacDonald RN, Buck WH, Su ACL, Harrell JR,
Mulhaupt R, Anderson BC (1989) Macromolecules 22:3851–3858.8. Mallin DT, Rausch MD, Lin YG, Dong S, Chien JCW (1990) J Am Chem Soc
112:2030–2031.9. Dietrich U, Hackmann M, Rieger B, Klinga M, Leskela M (1999) J Am Chem
Soc 121:4348–4355.10. Coates GW, Waymouth RM (1995) Science 267:217–219.11. Doi Y, Keii T (1986) Adv Polym Sci 73�74:201–248.
12. Tian J, Hustad PD, Coates GW (2001) J Am Chem Soc 123:5134–5135.
13. Saito J, Mitani M, Mohri J, Ishii S, Yoshida Y, Matsugi T, Kojoh S, KashiwaN, Fujita T (2001) Chem Lett, 576–577.
14. Furuyama R, Saito J, Ishii S, Makio H, Mitani M, Tanaka H, Fujita T (2005)J Organomet Chem 690:4398–4413.
15. Busico V, Cipullo R, Friederichs N, Ronca S, Talarico G, Togrou M, Wang B(2004) Macromolecules 37:8201–8203.
16. Mason AF, Coates GW (2004) J Am Chem Soc 126:16326–16327.17. Harney MB, Zhang YH, Sita LR (2006) Angew Chem Int Ed 45:2400–2404.18. Cherian AE, Rose JM, Lobkovsky EB, Coates GW (2005) J Am Chem Soc
127:13770–13771.19. Ruokolainen J, Mezzenga R, Fredrickson GH, Kramer EJ, Hustad PD, Coates
GW (2005) Macromolecules 38:851–860.20. Bates FS, Fredrickson GH, Hucul D, Hahn SF (2001) AIChE J 47:762–765.21. Brown GM, Butler JH (1997) Polymer 38:3936–3945.
15332 � www.pnas.org�cgi�doi�10.1073�pnas.0602894103 Hotta et al.